Influence of surface layer on mechanical and corrosion properties
of nickel-titanium orthodontic wires
Visnja Katica; Helena Otmacic Curkovicb; Damir Semenskic; Gorana Barsicd;Katarina Marusice; Stjepan Spaljf
ABSTRACTObjective: To analyze the effect of various coating formulations on the mechanical and corrosionproperties of nickel-titanium (NiTi) orthodontic wires.Materials and Methods: Uncoated, rhodium-coated, and nitrified NiTi wires were observed witha three-point-bend test, surface roughness (Ra) measurement, scanning electron microscopy,energy dispersive spectroscopy, and electrochemical testing (open circuit potential, electrochem-ical impedance spectroscopy, and cyclic polarization scan). Differences in the properties of testedwire types were analyzed with analysis of variance and Tukey post hoc test.Results: Uncoated and nitrified NiTi wires showed similar mechanical and anticorrosive properties,while rhodium-coated NiTi wires showed the highest Ra and significantly higher modulus ofelasticity, yield strength, and delivery of forces during loading but not in unloading. Rhodium-coatedNiTi wires also had the highest corrosion current density and corrosion potential, lowest impedancemodulus, and two time constants on Bode plot, one related to the Rh/Au coating and the other tounderlying NiTi.Conclusion: Working properties of NiTi wires were unaffected by various coatings in unloading.Nitrification improved corrosion resistance. Rhodium coating reduced corrosion resistance andpronounced susceptibility to pitting corrosion in artificial saliva because of galvanic couplingbetween the noble coating and the base alloy. (Angle Orthod. 2014;84:10411048.)
KEY WORDS: NiTi; Surface coating; Three-point-bend test; Corrosion; Electrochemical testing
Nickel-titanium (NiTi) orthodontic archwires possessboth shape memory and superelastic properties, andtheir low constant forces during a longer period of timeare considered to be desirable for tooth movement.1,2
Although there has been much research on basic wiretypes used in orthodontic therapy, every day we meetwith novel modifications of those basic materials thatare still insufficiently investigated.37 Changes insurface composition (for improved esthetic or reducedfriction) could affect wires roughness parameters8,9
and working and corrosive properties,1013 and as aresult, archwires could behave differently within theoral cavity.14,15 The surface roughness of archwires inorthodontics is still considered a controversial param-eter as far as its relation to friction and corrosion areconcerned as well as its relation to clinical use.5,1618
Uncoated NiTi wires have titanium oxides (TiOx) asanticorrosive components; rhodium-coated NiTi (RhNiTi) has gold and rhodium in a 0.5-mm thin layer (asstated by the manufacturer). Both are noble metalsand form a protective surface layer. Nitrified NiTi
a Research Assistant, Department of Pediatric Dentistry andOrthodontics, School of Medicine, University of Rijeka, Rijeka,Croatia.
b Assistant Professor, Department of Electrochemistry, Fac-ulty of Chemical Engineering and Technology, Zagreb, Croatia.
c Professor and Chair, Department of Experimental Mechan-ics, Faculty of Mechanical Engineering and Naval Architecture,Zagreb, Croatia.
d Research Assistant, Department of Precise Measurement,Faculty of Mechanical Engineering and Naval Architecture,Zagreb, Croatia.
e Research Assistant, Department of Electrochemistry, Facul-ty of Chemical Engineering and Technology, Zagreb, Croatia.
f Assistant Professor, Department of Pediatric Dentistry andOrthodontics, School of Medicine, University of Rijeka, Rijeka,Croatia.
Corresponding author: Visnja Katic, Kresimirova 40, HR-51000Rijeka, Croatia(e-mail: firstname.lastname@example.org)
Accepted: February 2014. Submitted: September 2013Published Online: March 21, 2014G 2014 by The EH Angle Education and Research Foundation,Inc.
DOI: 10.2319/090413-651.1 1041 Angle Orthodontist, Vol 84, No 6, 2014
(N NiTi), through the process of nitrogen ion implan-tation, forms titanium nitride (TiN) on the surface,replacing allergenic nickel with nitrogen. Previousstudies of TiN coating, produced experimentally inlaboratory conditions, showed improvement of me-chanical and biocompatible properties.19,20 Exact dataon the manufacturing process and conditions thecoated wires investigated herein were not availablefrom the manufacturer.
The corrosion of orthodontic wires in contact withsaliva is indeed an electrochemical process. It iscommon to perform in vitro studies of corrosionprocesses using electrochemical methods57,17,18,21,22
because the release of metal ions within the oralcavity occurs over a long period and is associated withdiscoloration of adjacent structures and teeth as wellas allergic and toxic reactions.14,15 Electrochemicalimpedance spectroscopy (EIS) testing determines thepolarization resistance, a direct measure of corrosionresistance; cyclic polarization testing helps in theobservation of the pitting tendencies of the alloy; andin vitro anodic polarization studies simulate the naturalcorrosion mechanism that usually happens over aprotracted duration of time. With all of these reasonstaken into account, clinicians should be informed aboutlimitations and potential risks when using variousmaterials.
Mechanical behavior, surface roughness, and anti-corrosive potential in commercially available orthodon-tic NiTi wires with various coatings are investigated inthis research. The hypotheses are that variouscoatings (1) do not affect mechanical properties, (2)change surface roughness parameters, and (3) im-prove anticorrosive properties of NiTi wires.
MATERIALS AND METHODS
Three types of preformed superelastic NiTi alloyorthodontic archwires (nickel, 50.4%; titanium, 49.6%),in dimensions of 0.020 3 0.020-inch BioForce Sentalloy(Dentsply GAC Int, Islandia, NY), were investigated:
N NiTi with untreated surfaceN Rh NiTi (High Aesthetic)N N NiTi (IonGuard)
Energy-dispersive spectroscopy was used to deter-mine the chemical composition of the surface and nearsurface of the wires (QUANTAX EDS, Bruker, Karls-ruhe, Germany) and to explore differences in brightand dark areas. The micromorphology of the surface ofone as-received and one electrochemically tested wireof each wire type was observed with field-emissionscanning electron microscopy (SEM) VEGA 3 (TESCAN,Brno, Czech Republic) at 20003 magnification.
Ten specimens, each 2.5-cm long, were cut from thestraight ends of archwires for every wire type and usedfor a three-point bending test. The support span ofTexture Analyser TA.HD.plus (Stable Micro Systems,Godalming, UK) was set to 12 mm and loaded with alow-force cell (5 kg, factory calibrated), according tocurrent standards.23,24 The temperature in a thermalchamber during measurements was set to 37uC with thehelp of a thermal coil and regulated automatically viathermal sensor. Each specimen was loaded to adeflection of 3.1 mm and then unloaded to zerodeflection at a cross-head speed of 0.0167 mm/s. Load,in Newtons (N), and deflection, in millimeters (mm),were collected every 5 milliseconds for both loading andunloading of each specimen using the Texture Expo-nent software program (Stable Micro Systems). Fromthe hysteresis loop, the following data were read off:loading and unloading elastic modulus (E) and yieldstrength (YS); analysis of forces in distances of 0.5, 1,1.5, 2, 2.5, and 3 mm during loading and unloading; andunloading slope characteristics (average plateau force,average plateau length, and the percentage of useableconstant force during unloading).
Measurement of surface roughness was performedusing the Stylus instrument Perthometer S8P (MahrGmbH, Gottingen, Germany). Traceability is assuredby using certified calibration artifacts (Croatian nationalroughness standards). Determination of roughnessparameter Ra was compliant with the geometricproduct specification standards (ISO 4287, 4288, and3274). Traced profiles of the real surface wereacquired with a diamond stylus of 5-mm radius. Duringthe measurement, the stylus was moved at a constantspeed across the samples with a measuring force of1.3 mN. Five randomly selected specimens from eachwire type were measured, and on each sample, Rawas measured on three profiles, using a Gaussian filterwith a cutoff value of 0.8 mm and the evaluation lengthof 4 mm. The arithmetic mean of three repeatedmeasurements was used for statistical analysis.
Specimens for corrosion testing were prepared fromhalved arch forms, each 50-mm long. Nail polish was
Table 1. Chemical Composition of Uncoated, Rhodium-Coated,
and Nitrified Nickel-Titanium Orthodontic Wires With Energy-
Dispersive Spectroscopy Analysis in As Received and After
Corrosion Test Conditions
Chemical Composition, wt %
Wire Type Ni Ti Rh Au N
Uncoated, as received 53.0 47.0
Uncoated, after test 51.2 48.8
Rh coated, as received 11.3 10.4 33.7 44.6
Rh coated, after test, bright spot 6.1 4.0 44.3 45.6
Rh coated, after test, dark spot 43.4 48.4 8.2
Nitrified, as received 52.3 46.8 0.9
Nitrified, after test 51.5 46.3 2.2
1042 KATIC, CURKOVIC, SEMENSKI, BARSIC, MARUSIC, SPALJ
Angle Orthodontist, Vol 84, No 6, 2014